Abstract
The miniaturization of integrated optical circuits below the diffraction limit for highspeed manipulation of information is one of the cornerstones in plasmonics research. By coupling to surface plasmons supported on nanostructured metallic surfaces, light can be confined to the nanoscale, enabling the potential interface to electronic circuits. In particular, gap surface plasmons propagating in an air gap sandwiched between metal layers have shown extraordinary mode confinement with significant propagation length. In this work, we unveil the optical properties of gap surface plasmons in silver nanoslot structures with widths of only 25 nm. We fabricate linear, branched and crossshaped nanoslot waveguide components, which all support resonances due to interference of counterpropagating gap plasmons. By exploiting the superior spatial resolution of a scanning transmission electron microscope combined with electron energyloss spectroscopy, we experimentally show the propagation, bending and splitting of slot gap plasmons.
Introduction
Manipulating the flow of electromagnetic waves on the nanoscale has been envisioned as the solution to interface nanometresized electronic circuits with diffractionlimited optical waveguides. For nanoscale control, the most promising approach is to couple propagating electromagnetic waves in dielectric media, such as optical fibres, to surfaceplasmon waves supported on nanostructured metallic surfaces^{1,2,3}. Surface plasmons are collective oscillations of the free electrons, and being confined to the metal surface they have the ability to localize light greatly beyond the diffraction limit and down to dimensions that bridge optoelectronics to electronic integrated circuits^{4}. A plethora of surfaceplasmon modes exists, which may be divided into two overall classes: localized surfaceplasmon resonances in confined nanoparticles and propagating surface plasmons in extended waveguides. Given its propagating nature, the latter is an ideal candidate for light manipulation on the nanoscale in integrated optical nanocircuits that can perform functions such as highspeed processing, routing or modulation^{5,6}.
While there are many different types of propagating surface plasmons^{4}, including nanoparticle chains^{7}, longrange surface plasmons^{8}, graphene plasmons^{9} and hybrid plasmonic–photonic modes^{10}, it is of paramount importance for nanocircuitry applications that the informationcarrying plasmonic mode has strong mode confinement with significant propagation length. In addition, properties such as singlemode operation and broadband guiding are needed. Despite the fundamental plasmonic tradeoff between mode confinement and propagation length^{11}, gap surface plasmons (GSPs), which propagate in a dielectric medium or air gap between metal surfaces^{12,13}, provide the required strong mode localization and micrometre propagation lengths^{14}, making them suitable for integrated optics. Guiding of GSPs has been experimentally realized in several different geometries^{15}, such as Vgrooves^{16}, slot waveguides^{17,18,19,20,21} and metal–insulator–metal (MIM) waveguides^{22}. So far, one of the most promising GSPbased waveguides for subwavelength circuitry has been the slot waveguide^{5,6,18,19}. Theoretical investigations^{23,24,25,26} of narrow slot waveguides have provided strong evidence for the aforementioned desired modal properties of the slot GSP, as well as an expected tolerance to fabrication imperfections and high transmittance through sharp bends^{27}. The slot GSP is therefore theoretically expected to be an ideal candidate for optical nanocircuitry, which we support experimentally in this work.
Characterizing the modal properties of the extremely confined GSP mode in nanosized slot waveguides using optical techniques, including even nearfield measurements^{20}, is a next to impossible task due to limited spatial resolution. In contrast, electron energyloss spectroscopy (EELS) performed in a scanning transmission electron microscope (STEM) can probe plasmonic response on the nanoscale^{28,29}. STEM EELS is a powerful characterization tool due to the combination of Angstrom spatial resolution with millielectronvolt spectral resolution over a broad energy range^{30,31}. In recent years, STEM EELS has proved to be an indispensable tool for optical characterization^{28} and has been utilized in many diverse plasmonic studies^{32,33,34,35,36,37,38,39,40,41,42,43,44}.
In this work, we use STEMEELS to characterize the GSP mode supported by freely suspended silver (on silicon nitride) slot waveguide resonators of only 25 nm width, which is several times narrower than stateoftheart slot waveguides^{6,18,19}. We study both straight and branched slot waveguide resonators for nanocircuitry applications. Besides providing experimental evidence for the important broadband propagation properties of the slot GSP, we also show that 90° bending with negligible back reflection can be achieved, which is required for nanoscale light routing. Light modulation often requires the splitting and interfering of several beams, which in both cases occurs at junctions in the optical circuit. By examining cross and Tshaped junctions in the slot waveguide resonators, we show that splitting can also be achieved with the slot GSP. On another note, the spectral positions of the GSPinduced excitations of the slot resonator depend strongly on the optical path length, which can be exploited for refractive index sensing. In fact, we show that the sensitivity of our nanoscale resonator is comparable to stateoftheart plasmonic sensors of similar footprints^{45}. The ease of fabrication and the desirable optical properties make the slot GSP of both fundamental and practical interest with a wide variety of plasmonic applications.
Results
Sample preparation
The samples are prepared by first depositing a silver film on a 10 nm thick silicon nitride transmission electron microscope (TEM) membrane. Slot geometries of different shape are subsequently fabricated by milling both the silver film and the silicon nitride substrate using a focused ion beam (FIB), see Fig. 1a for a schematic illustration of a straight slot waveguide resonator. As the lateral confinement (that is, in the y direction) of light is crucial for miniaturization of integrated optical circuits, the width of the slots should be as narrow as possible, that is, at the resolution limit of the FIB. The lateral spatial resolution of the FIB procedure and the ability to mill vertical side walls in the slot degrades with increasing silver film thickness t, making the deposition of a very thin silver film attractive. However, we must simultaneously ensure that the GSP supported by the slot should have the same favourable properties as that of the MIM GSP (corresponding to an infinitely thick silver film), such as strong mode localization, significant propagation length in a broad spectral range and singlemode operation. To this end, we have numerically verified that the effective index of the slot GSP mode for a thickness of t=150 nm (Supplementary Fig. 1) provides the desired modal properties along with ease of fabrication, which is why this thickness of the silver layer is chosen for the experimental study.
To study the guiding, bending and splitting of light on the nanoscale, we choose to fabricate straight, Lshaped and Tshaped slot resonators, respectively. Planview TEM images of selected fabricated structures can be seen in Fig. 1b–d. Here we see that all of the slots are extremely narrow with widths w of ∼25 nm, a size limited by the resolution of the FIB procedure. Expectedly, the width decreases in vicinity of the slot terminations, while at corners and junctions it becomes slightly larger. For the straight and Lshaped slot resonators (Fig. 1b,c), a total resonator length of ∼500 nm is chosen. While the branches of the Lshaped slot resonator in Fig. 1b are each ∼250 nm, we have also fabricated other Lshaped resonators with different branch sizes while keeping the total resonator length fixed at ∼500 nm. Finally, the Tshaped slot resonator shown in Fig. 1d has an upper branch of length 500 nm and a lower branch of ∼250 nm. Tshaped resonators with shorter lower branch lengths (approximately 125 and 170 nm) have also been fabricated and characterized. Importantly, as all of the prepared slot structures are on the same TEM membrane, the EELS characterization of all resonators can be carried out in the same microscope session (see Methods section), thereby eliminating any uncertainties associated with realignment between measurements of different resonators.
Straight slot
We begin by studying the subwavelength plasmon guiding properties of the slot by considering a straight slot waveguide resonator of length L≈500 nm and width w≈25 nm, see Fig. 2a for the STEM image. To map all of the plasmon modes supported by the slot, we record EELS data over a rectangular grid covering the entire slot (blue line in Fig. 2a) with a pixel size of ∼2 nm (see Methods for details). With this technique, usually referred to as spectrum imaging^{32}, we end up with a data cube with two spatial indices and one energy index. By summing over the two spatial indices, we end up with a single positionindependent EELS spectrum, shown in Fig. 2b, which contains loss events from all of the plasmon modes of the slot. Figure 2b displays five distinct resonances, where the three lowerenergy resonances are less pronounced than the two higherenergy resonances at 3.29 and 3.57 eV, indicating that the plasmon modes producing the latter resonances are more easily coupled to by the electron beam. Due to the positiveenergy tail of the immense zeroloss peak^{46}, the resonance at ∼0.75 eV is visible only as a weak shoulder. For further insight into the mode characteristics of each resonance, we visualize the spatial distribution of the EELS signal in a spectral window of 0.15 eV energy width centred at the resonance energy. Such an EELS intensity map for the resonance energy E=1.45 eV is shown in Fig. 2c, where an increased EELS signal is observed at specific positions in the air gap (boundary shown as a lightblue line). Interestingly, the EELS pattern is harmonic along the x direction near the upper and lower air–silver interfaces, indicating that the excited plasmon mode resides in the gap and propagates along the x direction. Such harmonic EELS patterns have also previously been observed in the study of complementary structures, which illustrate Babinet's principle^{47,48,49}. To highlight the plasmon propagation, we average the EELS signal in the air gap transverse to the propagation direction (that is, in the y direction), producing the onedimensional EELS line profile in Fig. 2d, which shows a clear harmonic pattern with two maxima. Proceeding in an identical manner with the EELS intensity maps for the resonance energies 2.03 and 2.53 eV produces the harmonic line profiles with three and four maxima in Fig. 2e,f, respectively. We interpret the harmonic patterns of Fig. 2d–f as standingwave resonances due to counterpropagating slot GSPs in the resonator (see also Supplementary Fig. 2 for the dispersion relation), although we note that the EELS pattern cannot directly be interpreted as the electric field profile^{50}. Instead, as we will see from later theoretical considerations, the EELS pattern can be understood as the GSP excitation efficiency of the electron. Finally, we consider in Fig. 2g,h the EELS intensity maps for the resonance energies 3.29 and 3.57 eV, respectively. Here we note that the two EELS intensity maps are quite similar to each other with a strong EELS signal near the air–silver boundary, but different from the harmonic pattern observed in the lowerenergy resonances. This suggests that the plasmon modes of these two resonances are similar in nature, but distinct from the GSPinduced resonances. Indeed, this difference in mode characteristic is emphasized when averaging the EELS intensity maps along the longitudinal direction (that is, x direction), where it becomes evident that the EELS signal of the GSPinduced resonances is maximized inside the air gap several nanometres from the air–silver boundary, while the maximum EELS signal of the highenergy plasmon modes is observed exactly at the air–silver boundary (Supplementary Fig. 3). By calculating the EELS response from electronexcited surface plasmons at planar silver–air and silver–silicon nitride–air interfaces in the nonretarded limit (Methods), we find the EELS signal shown in green and red lines in Fig. 2b, respectively. A single resonance appears in each case, which match in energy with our observed highenergy resonances. Thus, we interpret these two resonances as due to the coupling of the electron beam to the usual surface plasmons at the top (silver–air) and bottom (silver–silicon nitride–air) interfaces of our sample, as schematically illustrated in Fig. 1a. The significant thickness of the silver film (∼150 nm) gives rise to negligible hybridization of the planar surface plasmons, allowing us to model them individually. As the z component of the electric field of the planar surface plasmons is considerably stronger than that of the slot GSP, this interpretation also explains the much larger EELS signal observed from the surfaceplasmon modes compared to the slot GSPs. As our interest is only in the slot GSP, we continue with a focus on the EELS data below 3 eV.
To understand the experimental EELS data of the GSPinduced resonances, we complement the experimental results with theoretical considerations. Although there exists several approaches to calculating the EELS signal by solving the retarded Maxwell's equations in a particular geometry^{37,40,51,52,53,54}, we are primarily interested in the physical mechanism of the resonances and therefore adopt a simpler, yet accurate approach to determining the EELS signal. We model the resonator as a onedimensional slit of length L surrounded by silver and with effective index n_{eff}(w), which depends on the slit width w. The electron beam is for simplicity assumed to act as a point source, which generates forward and backwardpropagating GSP waves described as plane waves with wave number k=(ω/c)n_{eff} (Supplementary Note 1; Supplementary Fig. 4). By tracking the propagation and reflection of the GSP waves in the slot, we calculate the induced electric field in the slot and, hence, the EELS signal Γ(x_{0}, ω) as (Supplementary Note 1)
In equation (1), r denotes the complex reflection coefficient at the slotsilver terminations and x_{0} is the electron position in the slot (0<x_{0}<L). Thus, with a simple onedimensional model of the slot accounting for the counterpropagating GSP waves we arrive at equation (1), which describes both the position and frequencydependent EELS signal associated with Fabry–Perot resonances in the finitelength slot. To compare with our experimental EELS data in Fig. 2b, we also calculate the positionaveraged EELS signal Γ(ω) as
where we see that the resonance condition for the GSPinduced modes is . In fact, by rewriting this relation as 2kL+2arg(r)=2mπ, where arg(r) is the phase accumulation upon reflection and m is a positive integer, it becomes clear that resonance occurs when the accumulated roundtrip phase equals an integer value of 2π, like it is the case for any other Fabry–Perot problem. Although the width of the slot enters through the wave number k, the main geometric parameter determining the resonance condition is the resonator length L. In addition, we note that the parameter m describes the mode number by relating to the number of maxima in the standingwave pattern of the EELS signal, meaning that, for example, the m=1 mode corresponds to a standingwave pattern with one maximum.
To utilize equations (1) and (2), we approximate the reflection coefficient with the Fresnel reflection for a normallyincident plane wave
where is the complex refractive index of silver taken from literature^{55}. Finally, the GSP effective index is approximated by the analytical relation for the GSP mode of the metalinsulatormetal (that is, infinite thickness t→∞) geometry^{14,15}
which is valid for w>2/(k_{0}ɛ_{Ag}), appropriate for our structures. By comparison with numerical simulations of the effective index of the GSP mode of the finitethickness (t=150 nm) slot, we find that equation (4) accurately describes the effective index up to an energy of ∼2.5 eV (Supplementary Note 1; Supplementary Fig. 1). For energies above 2.5 eV, both the real and imaginary parts of the effective index of the finitethickness slot GSP mode increase markedly and can no longer be described by the simple relation in equation (4). Notably, most of the experimentally observed resonances occur below this energy, justifying our use of the analytical MIM relation to approximate the GSP mode of the slot. Hence, with equations (3) and (4) we can now analytically calculate the GSPinduced EELS spectrum and EELS intensity maps by using equations (2) and (1), respectively.
Figure 2b compares the theoretical EELS spectrum (equation (2)) with the experimental data, where we see that the analytical GSP model accurately captures the GSPinduced resonances observed experimentally. Impressively, the resonance energies for the two first GSP modes match almost exactly with measurements, although the firstorder GSP mode (m=1) is only weakly observed as a shoulder at approximately E=0.75 eV. For increasing resonance energies (that is, m=3 and m=4), the model predicts slightly larger energies than observed experimentally, which is to be anticipated from the approximative nature of equation (4). Besides the resonance energies of the GSPinduced modes, the analytical GSP model also displays a decreasing resonance amplitude and increasing fullwidth at halfmaximum with increasing mode number. Both features are in good agreement with experimental observations, except for the mode m=1, which is masked due to the strong background EELS signal at low energies. Finally, we note that the experimentally measured resonances appear spectrally broader than predicted by our analytical model. We attribute this difference in linewidth primarily to the limited energy resolution of EELS (0.10 eV) along with an increased imaginary part of the permittivity in silver due to gallium ion implantation from the FIB milling.
In addition to the spectral behaviour of the EELS signal, we also compare the spatial modal distribution of our analytical GSP model with the transversally averaged EELS signal in Fig. 2d–f. Evaluating equation (1) at the GSPinduced resonance energies produces the grey lines shown in Fig. 2d–f, which accurately captures the spatial distribution of the GSPinduced modes. Only for the case of m=4, that is, at the resonance energy 2.53 eV, do we observe a slight discrepancy in plasmon wavelength near the slot terminations. This can again be related to the only approximate relation in equation (4) at large energies, which also influences the calculation of the reflection coefficient. Besides this slight discrepancy, the analytical GSP model is impressively accurate and it is transparently describing both the spectral and spatial dependence of the EELS signal. The analytical GSP model also verifies that the experimentally observed resonances and EELS intensity maps are indeed consistent with the interpretation of counterpropagating slot GSPs producing standingwave patterns in a Fabry–Perot manner. Thus, the resonances at 1.45, 2.03 and 2.53 eV along with the weak shoulder at ∼0.75 eV are strong experimental evidences for the broadband singlemode GSP guiding property of the ultranarrow slit, covering almost the entire visible and nearinfrared spectral range.
The analytical GSP model provides an additional important point linked to the general interpretation of EELS, which we discuss briefly. Since the electron beam is modelled as a point source producing GSP waves, the EELS signal is then a measure of the efficiency of the electron beam to excite GSP modes in the resonators. Hence, a large EELS signal can be understood as a strong coupling between the electron beam and the GSP mode. This interpretation of EELS supplements the previously established understanding of EELS as related to the photonic local density of states^{50,56}. However, this interpretation also implies that the EELS intensity maps, that is, spatial EELS profiles, cannot simply be understood as the plasmonic mode profile^{32,33}. In particular for the slot GSP in this study, the main x and y electricfield components of the GSP have a different spatial dependence than the EELS intensity maps of Fig. 2c–f (Supplementary Fig. 1). Hence, the spatial EELS profiles should not be regarded as the GSP mode profiles, but rather as a map of the GSP excitation efficiency of the swift electrons during their interaction with a nontrivial superposition of the dispersive GSP modes.
Lshaped slot
One of the important requirements for a plasmonic mode to be suitable for nanoscale integrated circuits is a high transmission through sharp bends, that is, low back reflection, such that routing of light to desired locations can be achieved. We therefore characterize the bending property of the slot GSP mode by considering a slot resonator of similar length and width as the one in Fig. 2, but with a 90° bend in the middle of the resonator, see the inset of Fig. 3a for the STEM image. Given the symmetry of the Lshaped resonator in Fig. 3a, it is sufficient to consider only the EELS signal from one of the branches to map all of the modes. Figure 3a displays the EELS signal for the lower branch, where we observe four distinct resonances at energies 0.78, 1.40, 2.12 and 2.41 eV. All four energies are similar in value to the resonance energies observed for the straight slot resonator (Fig. 2), although the lowestenergy resonance was previously only observed as a weak shoulder. Hence, we anticipate these modes to be induced by counterpropagating slot GSPs with a similar propagation length L as for the case of the straight slot resonator, suggesting that the slot GSP bends around the 90° corner without significant back reflection or phase change. This interpretation is confirmed when examining the spatial distribution of the EELS signal, as shown in Fig. 3b–e. Once again, by averaging the EELS signal in the air gap transversally to the GSP propagation direction (see Methods for details), we extract onedimensional EELS profiles, which clearly show the expected standingwave pattern produced by the slot GSPs. For simplicity, we approximate the geometry of the waveguide bend by a 90° circular arc, whose radius can be regarded as the curvature of the bend. From inspection of the STEM image in the inset of Fig. 3a the radius of curvature is roughly 45 nm. The negligible back reflection from the corner seen in the Lshaped resonator of Fig. 3 has also been observed in other Lshaped resonators of similar total length (L≈500 nm), but with 90° bends positioned differently such that the branches have different lengths (data not included). In these cases, we also observe a very similar spectral and spatial EELS behaviour, confirming the high transmission of the slot GSP through sharp bends.
The low back reflection at the corner justifies the comparison of the experimental results of the Lshaped resonator with the analytical GSP model, which is based on a straight slot. Indeed, Fig. 3a displays accurate spectral agreement between the observed and calculated resonance energies, with the same decrease in accuracy of the theoretical model for larger energies (as a consequence of the validity of equation (4)). Comparison of spatial EELS profiles (Fig. 3b–e) also shows good agreement between theory and experiments, although we note that the EELS signal drops at the corner, which is more pronounced for the modes with standingwave patterns that have maxima at the corner (that is, m=1 and m=3). In particular, the lowestorder mode (m=1) shows this effect in Fig. 3b. We observe the same phenomenon at Tshaped junctions, which we discuss later, and crossshaped junctions (Supplementary Fig. 5). Ruling out FIBinduced silver modification at the corners (Supplementary Fig. 6), we interpret the decreased EELS signal to be a consequence of the decreased GSP excitation efficiency of the electron beam. We relate this effect to (i) the weaker charge distribution due to the lack of a direct opposing metal boundary (compared with the straight sections) and (ii) the decreased local GSP effective index (due to an increased width), providing less mode confinement and weaker electric field components. The increase in slot width also decreases the averaged EELS signal. Disregarding the cornerrelated decrease in EELS signal, we find once again excellent agreement between experiments and the analytical GSP model. More importantly, we have successfully showed the bending property of the slot GSP with negligible bending loss and high transmission.
Tshaped slot
Nanoscale onchip modulation of light requires the interference or splitting of one or several beams at junctions in the waveguide circuit. Hence, understanding the behaviour of the slot GSP at junctions is essential for constructing a plasmonic circuit. We have therefore fabricated a Tshaped slot resonator, as shown in the inset of Fig. 4a, with upper and lower branch lengths of approximately 500 and 250 nm, respectively. The EELS signal from the upper and lower branches is shown in Fig. 4a in blue and red lines, respectively. Here we note the striking resemblance of the two EELS spectra. In particular, both branches show four GSPinduced resonances at the energies 0.79, 1.54, 2.13 and 2.59 eV. We also note that these resonance energies are similar to those observed in the Lshaped and straight slot resonators. The similarity in resonance energies of the two branches and the two other resonators are a consequence of the similar propagation length, leading to almost identical resonance conditions. A total length of ∼500 nm is traversed by the slot GSP regardless if the path is the upper branch only, or if the path, by splitting of the GSP, includes half of the upper branch and the lower branch. In other words, the two different paths give rise to degenerate GSPinduced resonances. The fact that no new GSPinduced resonances are observed, which reside only in the lower branch, is evidence for the splitting of the slot GSP at the Tshaped junction with minimal reflection. The transversally averaged spatial EELS profiles of the GSPinduced resonances in the upper branch are shown in Fig. 4b–e, which show the expected standingwave patterns with increasing number of maxima (Supplementary Fig. 7 for the EELS profiles through the junction). Comparison with the analytical GSP model shows accurate spectral and spatial agreement, although the spatial profiles for the oddnumbered modes m=1 and m=3 differ at the junction. As discussed in relation to the Lshaped resonator, the experimentally observed dip in the EELS signal at the junction is a consequence of the decrease in GSP excitation efficiency of the electron, which is not accounted for in the analytical GSP model.
We can lift the degeneracy of the GSPinduced modes by changing the length of the lower branch in the Tshaped resonator, such that the two different paths have different lengths and thereby resonate at different energies. We consider this case in Fig. 5a, where we show the EELS signal from a Tshaped resonator with a lower branch of shorter length (∼170 nm). Thus, the path along the upper branch still has a length of ∼500 nm, while the GSP path involving the lower branch is now around 390 nm. From Fig. 5a, we note that this difference in path length leads to different EELS response from the two branches. In total, we observe four resonances at energies 0.76, 1.05, 1.69, and 2.14 eV. On the basis of the spatial profiles in Fig. 5b,d, the resonances at 0.76 and 2.14 eV are immediately identified as the m=1 and m=3 modes related to counterpropagating slot GSPs in the upper branch (that is, L≈500 nm). Similar resonance energies for these modes were also previously observed for the straight and Lshaped resonators. The interesting features are the two remaining resonances, which differ in energy from any of the previous slot GSP resonances. By considering the spatial profile in Fig. 5e and comparing with the analytical GSP model, we interpret the resonance at energy 1.05 eV as the firstorder (m=1) GSPinduced mode associated with the shorter path (L≈390 nm). Surprisingly, for the resonance energy at 1.69 eV, we find that we can consider the spatial profile along both the long path (Fig. 5c) and the short path (Fig. 5f), showing in both cases two maxima. Interestingly, this suggests that the observed resonance is due to the hybridization of the secondorder GSP modes (m=2) of the short and long paths. Summarizing, we have provided strong evidence for splitting of the slot GSP at junctions, which even leads to resonant excitations at other energies (compared with the straight and Lshaped resonators) due to change in path lengths.
Discussion
The properties of the slot GSP, including propagation, bending, and splitting, have been thoroughly investigated by EELS characterization of ultracompact silver slot resonators. We have shown that the resonances in finitelength slots are primarily determined by the overall path length traversed by the slot GSP, regardless of bending around corners or splitting in junctions. In Fig. 6a, we emphasize this important point by comparing the EELS signal from straight, Lshaped, and Tshaped resonators. The Lshaped resonator has the corner situated ∼125 nm from the left slot termination (differing from the Lshaped resonator in Fig. 3), while the Tshaped resonator is the same as that in Fig. 5. Since the overall propagation distance of the slot GSP is ∼500 nm for the straight and the Lshaped slot resonators, the GSPinduced resonances occur at approximately the same energies. Hence, the slot GSP bends around the 90° corner effortlessly in a broad spectral range, making the GSPinduced resonant modes basically unaltered by the presence of the corner. In contrast, the introduction of a shorter path length in the Tshaped resonator (by splitting in the junction) gives rises to new resonances with, in this case, energies of 1.05 and 1.69 eV.
The dependence of the GSPinduced resonance energies on the lower branch length of the Tshaped resonator is investigated in more detail in Fig. 6b. Here we map the GSPinduced resonances by considering the EELS signal from the upper branch, which has a constant length of 500 nm in all three cases. The lower branch length increases from ∼125 nm through 170 to 250 nm. Here we clearly see that the first and secondorder (m=1 and m=2) modes related to the path length involving the lower branch decrease in resonance energy with increasing lower branch length (that is, overall path length). Hence, the GSPinduced resonances, as tracked from the upper branch, are extremely sensitive to the optical path length of the slot GSP. By straightforwardly converting the change in optical length of the lower branch into a change in refractive index while keeping the length fixed at 125 nm, we can estimate the sensitivity S of the Tshaped slot waveguide resonator, that is, the wavelength shift per refractive index unit (RIU). We find the refractive index sensitivities of the firstorder and secondorder modes to be S_{m=1}≈550 nm/RIU and S_{m=2}≈150 nm/RIU. Impressively, the sensitivity of the firstorder mode is comparable to stateoftheart plasmonic sensors of similar footprints^{45}, while being ultracompact with a volume of only ≈(0.5 × 0.15 × 0.15) μm^{3}=0.01 μm^{3}. Besides the sensitivity, another parameter for characterizing a sensor is the figureofmerit relating to the resonance linewidth^{45}. Unfortunately, accurate quantitative determination of plasmon linewidths with EELS is not readily possible due to the energy resolution of EELS, although progress in this direction has recently been achieved^{57,58}. Since the EELS signal is connected to the photonic local density of states^{56,59}, the marked changes in both the spatial and spectral EELS response of the upper branch can also be observed in the response of quantum emitters. Note that the GSP modes form the basis for the channel plasmon polaritons propagating along Vgrooves, that were recently demonstrated to be well suitable for efficient coupling to individual quantum emitters^{60}. Yet another perspective application of extremely confined GSP modes similar to those studied here can be their usage for resonant guided wave networks^{61,62}.
Overall, extremely confined GSP modes studied in this work exhibit remarkable flexibility in their manipulation, a unique feature that, in our opinion, opens up new avenues for their exploitation in diverse areas of modern nanophotonics, ranging from ultracompact resonators for refractiveindex sensing and resonant guidedwave networks to quantum plasmonics.
Methods
Fabrication
Commercially available silicon nitride TEM membranes (10 nm thickness) are used as a thin planar substrate. A 150 nm thick smooth silver film is then deposited onto the substrate using ebeam evaporation. Subsequently, different slot geometries are milled into the silver film using focused ion beam (FIB) with a FEI Helios 600i dual FIB/SEM tool.
Due to short periods of air exposure of the samples, we could not effectively prevent the oxidation or sulfidation of silver at the top interface of the sample. However, the airinduced changes to the top interface primarily affects the surface plasmon excited at the corresponding interface and thus have no significant impact on the gap surfaceplasmon modes.
EELS measurements
The EELS measurements are performed with a FEI Titan transmission electron microscope equipped with a monochromator and an image corrector. The microscope is operated in STEM mode at an acceleration voltage of 300 kV, providing a spot size of ∼0.3 nm and an energy resolution of 0.10 eV (measured as the fullwidth at halfmaximum of the zeroloss peak). The microscope is equipped with a Quantum 966 electron energyloss spectrometer and the Gatan DigiScan acquisition system, which records an entire EELS intensity map in 20 to 40 min, depending on the number of pixels. A C3 aperture size of 50 μm, camera length of 38 mm and entrance aperture of 2.5 mm were used for the EELS measurements. This correspond to convergence and collection angles of 8.4 and 18.3 mrad, respectively. A spectral dispersion of 0.01 eV per pixel was used in all of the spectra collection. In addition, we utilize the automatic drift and darkcurrent correction function included in the acquisition system. The individual EELS spectrum of the EELS intensity maps (with pixel sizes typically of 2–2.5 nm) are recorded with acquisition times ranging from 10 to 12 ms.
The first postprocessing step of the EELS spectra is the removal of the zeroloss peak using the reflectedtail method, where the negative energy part of the zeroloss peak is mirrored around the zeroenergy point to reconstruct the zeroloss peak and subsequently subtracted from the spectra. The resonance energies are then extracted by fitting a Gaussian function using a nonlinear leastsquares fit. All of the resonant EELS intensity maps shown in this paper depict the summed EELS signal in a 0.15 eV spectral window centred at the extracted resonance energies. In Fig. 6, we additionally subtract the background contribution to the EELS signal by fitting two linear functions; the first in the energy range 0.5 eV to around 1 eV and the second in the energy range from around 1 to 2.7 eV. Both linear fits are performed by manually excluding the data of the gap surfaceplasmon peaks.
To compare the EELS intensity maps at resonance with the onedimensional analytical GSP model, we convert the twodimensional EELS maps into onedimensional EELS line profiles using an averaging procedure. To increase the signaltonoise ratio, we use only the EELS data in the air gap of the GSP resonators. Thus, we initially determine the boundary between the air gap and the surrounding silver using the Image Processing Toolbox in MATLAB. By converting the greyscale STEM image into a binary image using the threshold determined from Otsu’s method, we extract the air–silver boundary. Subsequently, we average the EELS data within the closed boundary transversely to the GSP propagation direction. For the straight slot in Fig. 2, this approach amounts to averaging the EELS data along the y direction. However, for the resonators with bends and splits (L and Tshaped), we fit the corner with a 90° circular arc. Averaging the EELS data in a corner is then performed along straight lines perpendicular to the fitted arc (that is, in the radial direction). The radius of the fitted circular arc is also used as a measure for the radius of curvature of the fabricated bends.
Simulations
The derivation of the onedimensional analytical GSP model for calculating the EELS signal is presented in detail in Supplementary Note 1.
The EELS signal from the top and bottom surface plasmons (Fig. 2a) is calculated using a 2D model in COMSOL Multiphysics (version 5.1), where the electron beam is set to travel parallel to the metaldielectric interfaces. The electron beam is modelled as an outofplane line current with wave number k_{e}=ω/v, where v is the electron speed. Although the electron beam travels perpendicular to the metaldielectric interfaces in the experiments, our only interest is in evaluating the EELS signal stemming from the excitation of surface plasmons at their nonretarded frequencies. This can be achieved using the 2D implementation by setting a low electron velocity (here, v=0.5c) and positioning the electron beam to always travel in the vacuum part of the domain (a distance of 5 nm to the outer interface is chosen). In this manner, the main contribution to the theoretical EELS signal will be from the excitation of surface plasmons at their nonretarded energies, just as in the experiments. In all calculations, we use the permittivity for silver from ref. 55, while the permittivity for silicon nitride is from ref. 63. A thickness of 10 nm is used to model the silicon nitride layer from the TEM membrane.
Data availability
Data available on request from the authors.
Additional information
How to cite this article: Raza, S. et al. Electron energyloss spectroscopy of branched gap plasmon resonators. Nat. Commun. 7, 13790 doi: 10.1038/ncomms13790 (2016).
Publisher's note: Springer Nature remains neutral with regard to jurisdictional claims in published maps and institutional affiliations.
References
 1
Ozbay, E. Plasmonics: merging photonics and electronics at nanoscale dimensions. Science 311, 189–193 (2006).
 2
Zia, R., Schuller, J. A., Chandran, A. & Brongersma, M. L. Plasmonics: the next chipscale technology. Mater. Today 9, 20–27 (2006).
 3
Brongersma, M. L. & Shalaev, V. M. The case for plasmonics. Science 328, 440–441 (2010).
 4
Gramotnev, D. K. & Bozhevolnyi, S. I. Plasmonics beyond the diffraction limit. Nat. Photon. 4, 83–91 (2010).
 5
Melikyan, A. et al. Highspeed plasmonic phase modulators. Nat. Photon 8, 229–233 (2014).
 6
Haffner, C. et al. Allplasmonic MachZehnder modulator enabling optical highspeed communication at the microscale. Nat. Photon 9, 525–528 (2015).
 7
Maier, S. A. et al. Local detection of electromagnetic energy transport below the diffraction limit in metal nanoparticle plasmon waveguides. Nat. Mater. 2, 229–232 (2003).
 8
Berini, P. Longrange surface plasmon polaritons. Adv. Opt. Photon. 1, 484–588 (2009).
 9
Christensen, J., Manjavacas, A., Thongrattanasiri, S., Koppens, F. H. L. & García de Abajo, F. J. Graphene plasmon waveguiding and hybridization in individual and paired nanoribbons. ACS Nano 6, 431–440 (2012).
 10
Oulton, R. F., Sorger, V. J., Genov, D., Pile, D. & Zhang, X. A hybrid plasmonic waveguide for subwavelength confinement and longrange propagation. Nat. Photon 2, 496–500 (2008).
 11
Maier, S. A. Plasmonics: Fundamentals and Applications (Springer, 2007).
 12
Economou, E. N. Surface plasmons in thin films. Phys. Rev. 182, 539–554 (1969).
 13
Zia, R., Selker, M. D., Catrysse, P. B. & Brongersma, M. L. Geometries and materials for subwavelength surface plasmon modes. J. Opt. Soc. Am. A 21, 2442–2446 (2004).
 14
Bozhevolnyi, S. I. & Jung, J. Scaling for gap plasmon based waveguides. Opt. Express 16, 2676–2684 (2008).
 15
Smith, C. L. C., Stenger, N., Kristensen, A., Mortensen, N. A. & Bozhevolnyi, S. I. Gap and channeled plasmons in tapered grooves: a review. Nanoscale 7, 9355–9386 (2015).
 16
Bozhevolnyi, S. I., Volkov, V. S., Devaux, E., Laluet, J.Y. & Ebbesen, T. W. Channel plasmon subwavelength waveguide components including interferometers and ring resonators. Nature 440, 508–511 (2006).
 17
Dionne, J. A., Lezec, H. J. & Atwater, H. A. Highly confined photon transport in subwavelength metallic slot waveguides. Nano Lett. 6, 1928–1932 (2006).
 18
Kriesch, A. et al. Functional plasmonic nanocircuits with low insertion and propagation losses. Nano Lett. 13, 4539–4545 (2013).
 19
Huang, K. C. Y. et al. Electrically driven subwavelength optical nanocircuits. Nat. Photon 8, 244–249 (2014).
 20
Andryieuski, A. et al. Direct characterization of plasmonic slot waveguides and nanocouplers. Nano Lett. 14, 3925–3929 (2014).
 21
Gramotnev, D. K., Nielsen, M. G., Tan, S. J., Kurth, M. L. & Bozhevolnyi, S. I. Gap surface plasmon waveguides with enhanced integration and functionality. Nano Lett. 12, 359–363 (2012).
 22
Miyazaki, H. T. & Kurokawa, Y. Squeezing visible light waves into a 3nmthick and 55nmlong plasmon cavity. Phys. Rev. Lett. 96, 097401 (2006).
 23
Liu, L., Han, Z. & He, S. Novel surface plasmon waveguide for high integration. Opt. Express 13, 6645–6650 (2005).
 24
Pile, D. F. et al. Twodimensionally localized modes of a nanoscale gap plasmon waveguide. Appl. Phys. Lett. 87, 261114 (2005).
 25
Veronis, G. & Fan, S. Guided subwavelength plasmonic mode supported by a slot in a thin metal film. Opt. Lett. 30, 3359–3361 (2005).
 26
Shi, X. & Hesselink, L. Design of a C aperture to achieve λ/10 resolution and resonant transmission. J. Opt. Soc. Am. B 21, 1305–1317 (2004).
 27
Pile, D. F., Gramotnev, D. K., Oulton, R. F. & Zhang, X. On longrange plasmonic modes in metallic gaps. Opt. Express 15, 13669–13674 (2007).
 28
García de Abajo, F. J. Optical excitations in electron microscopy. Rev. Mod. Phys. 82, 209–275 (2010).
 29
Colliex, C., Kociak, M. & Stéphan, O. Electron energy loss spectroscopy imaging of surface plasmons at the nanometer scale. Ultramicroscopy 162, A1–A24 (2016).
 30
Krivanek, O. L. et al. Vibrational spectroscopy in the electron microscope. Nature 514, 209–212 (2014).
 31
Nicoletti, O. et al. Threedimensional imaging of localized surface plasmon resonances of metal nanoparticles. Nature 502, 80–84 (2013).
 32
Bosman, M., Keast, V. J., Watanabe, M., Maaroof, A. I. & Cortie, M. B. Mapping surface plasmons at the nanometre scale with an electron beam. Nanotechnology 18, 165505 (2007).
 33
Nelayah, J. et al. Mapping surface plasmons on a single metallic nanoparticle. Nat. Phys. 3, 348–353 (2007).
 34
Nelayah, J. et al. Direct imaging of surface plasmon resonances on single triangular silver nanoprisms at optical wavelength using lowloss EFTEM imaging. Opt. Lett. 34, 1003–1005 (2009).
 35
Koh, A. L., FernándezDomínguez, A. I., McComb, D. W., Maier, S. A. & Yang, J. K. W. Highresolution mapping of electronbeamexcited plasmon modes in lithographically defined gold nanostructures. Nano Lett. 11, 1323–1330 (2011).
 36
Nicoletti, O. et al. Surface plasmon modes of a single silver nanorod: an electron energy loss study. Opt. Express 19, 15371–15379 (2011).
 37
Duan, H., FernándezDomínguez, A. I., Bosman, M., Maier, S. A. & Yang, J. K. W. Nanoplasmonics: classical down to the nanometer scale. Nano Lett. 12, 1683–1689 (2012).
 38
Raza, S. et al. Blueshift of the surface plasmon resonance in silver nanoparticles studied with EELS. Nanophotonics 2, 131–138 (2013).
 39
Rossouw, D. & Botton, G. A. Plasmonic response of bent silver nanowires for nanophotonic subwavelength waveguiding. Phys. Rev. Lett. 110, 066801 (2013).
 40
Raza, S. et al. Extremely confined gap surfaceplasmon modes excited by electrons. Nat. Commun. 5, 4125 (2014).
 41
Martin, J. et al. Highresolution imaging and spectroscopy of multipolar plasmonic resonances in aluminum nanoantennas. Nano Lett. 14, 5517–5523 (2014).
 42
Tan, S. F. et al. Quantum plasmon resonances controlled by molecular tunnel junctions. Science 343, 1496–1499 (2014).
 43
Schoen, D. T., Atre, A. C., GarcaEtxarri, A., Dionne, J. A. & Brongersma, M. L. Probing complex reflection coefficients in onedimensional surface plasmon polariton waveguides and cavities using STEM EELS. Nano Lett. 15, 120–126 (2015).
 44
Raza, S. et al. Multipole plasmons and their disappearance in fewnanometer silver nanoparticles. Nat. Commun. 6, 8788 (2015).
 45
Anker, J. N. et al. Biosensing with plasmonic nanosensors. Nat. Mater. 7, 442–453 (2008).
 46
Egerton, R. F. Electron Energy Loss Spectroscopy in the Electron Microscope 3rd edn (Springer, 2011).
 47
Ögüt, B. et al. Hybridized metal slit eigenmodes as an illustration of Babinet's principle. ACS Nano 5, 6701–6706 (2011).
 48
von Cube, F. et al. Spatiospectral characterization of photonic metaatoms with electron energyloss spectroscopy [Invited]. Opt. Mater. Express 1, 1009–1018 (2011).
 49
Rossouw, D. & Botton, G. A. Resonant optical excitations in complementary plasmonic structures. Opt. Express 20, 6968–6973 (2012).
 50
Hohenester, U., Ditlbacher, H. & Krenn, J. R. Electronenergyloss spectra of plasmonic nanoparticles. Phys. Rev. Lett. 103, 106801 (2009).
 51
Ritchie, R. H. Plasma losses by fast electrons in thin films. Phys. Rev. 106, 874–881 (1957).
 52
Garca de Abajo, F. J. & Howie, A. Retarded field calculation of electron energy loss in inhomogeneous dielectrics. Phys. Rev. B 65, 115418 (2002).
 53
Bigelow, N. W., Vaschillo, A., Iberi, V., Camden, J. P. & Masiello, D. J. Characterization of the electron and photondriven plasmonic excitations of metal nanorods. ACS Nano 6, 7497–7504 (2012).
 54
Hohenester, U. & Trügler, A. MNPBEMA Matlab toolbox for the simulation of plasmonic nanoparticles. Comp. Phys. Commun. 183, 370–381 (2012).
 55
Johnson, P. B. & Christy, R. W. Optical constants of the noble metals. Phys. Rev. B 6, 4370–4379 (1972).
 56
García de Abajo, F. J. & Kociak, M. Probing the photonic local density of states with electron energy loss spectroscopy. Phys. Rev. Lett. 100, 106804 (2008).
 57
Bosman, M. et al. Surface plasmon damping quantified with an electron nanoprobe. Sci. Rep. 3, 1312 (2013).
 58
Bosman, M. et al. Encapsulated annealing: Enhancing the plasmon quality factor in lithographicallydefined nanostructures. Sci. Rep. 4, 5537 (2014).
 59
Christensen, T. et al. Nonlocal response of metallic nanospheres probed by light, electrons, and atoms. ACS Nano 8, 1745–1758 (2014).
 60
BermúdezUreña, E. et al. Coupling of individual quantum emitters to channel plasmons. Nat. Commun. 6, 7883 (2015).
 61
Feigenbaum, E. & Atwater, H. A. Resonant guided wave networks. Phys. Rev. Lett. 104, 147402 (2010).
 62
Burgos, S. P., Lee, H. W., Feigenbaum, E., Briggs, R. M. & Atwater, H. A. Synthesis and characterization of plasmonic resonant guided wave networks. Nano Lett. 14, 3284–3292 (2014).
 63
Philipp, H. R. Optical properties of silicon nitride. J. Electrochem. Soc. 120, 295–300 (1973).
Acknowledgements
S.I.B. acknowledges financial support by European Research Council, Grant 341054 (PLAQNAP). The Center for Nanostructured Graphene is sponsored by the Danish National Research Foundation, Project DNRF103. Sample preparation by FIB (FEI Helios NanoLab 600i) and sample characterization by TEM (FEI Titan) were performed at the Stanford Nano Shared Facilities (SNSF). The research at Stanford was supported by a Multi University Research Initiative (MURI FA95501210488).
Author information
Affiliations
Contributions
S.R. and M.L.B. conceived the idea. M.E. and S.R. fabricated the samples. A.L.K. and S.R. performed the EELS measurements. S.R. analysed the EELS data and the images. S.I.B., M.L.B., N.A.M. and S.R. interpreted the results. Writing of the manuscript was done in a joint effort.
Corresponding authors
Ethics declarations
Competing interests
The authors declare no competing financial interests.
Supplementary information
Supplementary Information
Supplementary Figures, Supplementary Note and Supplementary References (PDF 660 kb)
Rights and permissions
This work is licensed under a Creative Commons Attribution 4.0 International License. The images or other third party material in this article are included in the article’s Creative Commons license, unless indicated otherwise in the credit line; if the material is not included under the Creative Commons license, users will need to obtain permission from the license holder to reproduce the material. To view a copy of this license, visit http://creativecommons.org/licenses/by/4.0/
About this article
Cite this article
Raza, S., Esfandyarpour, M., Koh, A. et al. Electron energyloss spectroscopy of branched gap plasmon resonators. Nat Commun 7, 13790 (2016). https://doi.org/10.1038/ncomms13790
Received:
Accepted:
Published:
DOI: https://doi.org/10.1038/ncomms13790
Further reading

Nanoelectromechanical modulation of a stronglycoupled plasmonic dimer
Nature Communications (2021)

Spontaneous and stimulated electron–photon interactions in nanoscale plasmonic near fields
Light: Science & Applications (2021)

Lightdriven selfassembly of heteroshaped gold nanorods
Applied Physics A (2018)
Comments
By submitting a comment you agree to abide by our Terms and Community Guidelines. If you find something abusive or that does not comply with our terms or guidelines please flag it as inappropriate.